Influence of Planetary Ball Mill Parameters on Powder Flowability of AlSi10Mg with Niobium Carbide Using Central Composite Design (CCD)

School of Mechanical Engineering, SASTRA Deemed to Be University, anjavur 613401, Tamil Nadu, India Department of Mechanical Engineering, KPR Institute of Engineering and Technology, Coimbatore 641407, Tamil Nadu, India Department of Civil Engineering, Government Engineering College, Jhalawar 326023, Rajasthan, India Department of Mechanical Engineering, Government Engineering College, Jhalawar 326023, Rajasthan, India Department of Electrical Engineering, FET, MJP Rohilkhand University, Bareilly 243006, UP, India Department of Mechanical Engineering, Faculty of Manufacturing, Institute of Technology, Hawassa University, Hawassa, Ethiopia


Introduction
Metal-based additive manufacturing is an emerging technology that produces components within the stipulated period and achieves high dimensional accuracy [1]. Generally, this technology employs only a speci ed powder category, such as atomized particles, depending on the manufacturer's speci cation. e atomized powder properties must be addressed based on the processability criterion to ensure the component's print quality [2]. e properties of the powder comprise the owability, the density of the powder (apparent density and tapped density), particle shape (morphology), the powder synthesis process, and the particle size distribution (PSD) that a ect the building of the powder layer on the platform. e owability of the powder should be adequate for an e ective additive manufacturing process [3]. In processing aluminum alloys by additive manufacturing, the powder's morphology and size distribution play a decisive role in ensuring the material's packing density [4]. e particle shape signi cantly in uences good owability than the size distribution [5]. Ball milling is widely preferred for aluminum-based matrix composites to mix/blend the two different sizes and shapes of powders (matrix + reinforcement) in varying volumes or weight percentages following other optimization techniques.
Moreover, the ball mill's input parameters substantially affect the blended powder flow properties [6][7][8][9][10][11][12][13][14]. For the application of greater hardness, niobium carbide (NbC) is preferred among other transition metal carbides (TMC) due to its higher bulk modulus and incorporating an irregularshaped carbide as reinforcement improves the wear resistance of the matrix element [15,16]. e mixing of two different powders (metals as matrix and ceramic as reinforcement) with various morphologies was possible to process through casting [17] and powder metallurgy [18] routes for powder preparation. Compared to the previous routes, ceramic reinforcements (other TMCs) in the Albased matrix showed remarkable mechanical properties such as high hardness and high wear resistance [19] when compared to the base alloy through the selective laser melting (SLM) process and are suitable for tribological applications. Furthermore, compared to traditional approaches such as casting and powder metallurgy, composite fabrication via additive manufacturing has benefits in terms of design, freedom, and the ability to manufacture complicated designs [20]. However, it is challenging because of the additive manufacturing processability [21].
From a critical review of the literature, it was noted that the optimization of powder flow characteristics in the combination of hypoeutectic aluminum alloy (AlSi10Mg) and group VB transition metal carbide (NbC) was not explored much in the scope of additive manufacturing. erefore, evaluating the mixed powder characteristics of AlSi10Mg (spherical) and NbC (aggregate irregular) with varying weight percentages is required before being fed into the processing window of additive manufacturing. e objective of the work is to investigate the powder flowability characteristics of AlSi10Mg with the addition of NbC based on apparent density (AD), tapped density (TD), and static angle of repose (SAoR) values through regular mixing in a planetary ball mill following the central composite design approach. At the same time, the Hausner's Ratio (HR) and the Carr Index (CI) values resulted from the apparent and tapped densities of the mixed powder.

Materials and Methods
e AlSi10Mg powder (Si-10; Mg-0.35; Al-Balance; Supplier: Carpenter Additive, UK) of a mean particle size of 41.79 microns and NbC powder (99% Pure; Supplier: Alfa Aesar, UK) of a mean particle size of 12.05 microns were used. e AlSi10Mg was considered a matrix element in the experimental study, whereas the NbC was taken as particulate ceramic reinforcement. e morphology of procured AlSi10Mg with a spherical shape and NbC with an aggregate irregular shape was observed using a scanning electron microscope (Vega3 TESCAN) analysis, as shown in Figures 1(a) and 1(b). e X-ray photoelectron spectroscope ( ermo Fisher) analysis was carried out for procured powders, as shown in Figure 2, and no impurities were identified in either of the powder samples. Two powders were regularly mixed using a planetary ball mill with a single jar holder (VB Ceramic Consultants, India). For maintaining the spherical shape of the AlSi10Mg, the balls are not used during regular mixing. Using MINITAB (Version-18.0), the central composite design (CCD) was preferred in this investigation to analyze and optimize the planetary ball mill's input parameters to ensure the effects of extreme levels of factors involved. e three main input parameters for regular mixing using a planetary ball mill are time (hours), speed (RPM), and NbC composition (% weight), which play a vital role in predicting powder flowability. e input parameters and levels are shown in Table 1. Based on the three input factors and five levels of each factor, 20 sets of experiments were designed and included in Table 2. e scanning electron microscope (SEM) samples examined the morphology change of the master alloy and ensured the distribution of reinforcement in the matrix. e powder flow characteristics study was performed based on apparent density: ASTM B 212, tapped density: ASTM B 527 [22], static angle of repose: ASTM B213 [23], Hausner's Ratio: ASTM D7481-09, and Carr Index: ASTM D6393-14 [24].

Analysis of CCD Experiments.
e CCD was employed to predict the influence of the extreme limits of the input parameters such as time, speed, and composition on the output responses. Also, CCD was used for developing the mathematical model for the responses such as apparent density, tapped density, and static angle of repose. e apparent density and tapped density values were obtained by the Hall flowmeter method and mechanical tapping 50 times, respectively, conforming to the ASTM standards. Generally, the lower values of apparent and tapped densities exhibit the poor flowability of the powders. For the flowability indication of mixed powder, the HR and CI values were attained using (1) and (2). For better flowability, the lower Hausner's Ratio and Carr Index values were preferred. e static angle of repose of the mixed powder was attained using (3) based on the piling diameter and height, followed by the fixed cone height approach. e static angle of repose was used to assess the mixed powder's internal condition, such as cohesiveness or friction between the particles. More cohesiveness leads to an increased static angle of repose and affects the flow of the mixed powder. Table 3 shows the data of output responses based on the CCD experiments. In experimental analysis, the CCD experiments were classified into three categories, namely , center-based (E5, E6, E11, E18, E19, and E20), extreme-based (E3, E4, E9, E13, E16, and E17), and factor-based (E1, E2, E7, E8, E10, E12, E14, and E15). From Table 3, it was noted that experiments E4 and E9 show the worst flow characteristics based on the results of the output responses due to the mixing in extreme conditions like a more extended time (6.02 hours) and higher NbC composition (11.043% weight) under the rotational speed of 150 RPM.
Conversely, E8, E10, E12, E13, E14, and E15 show good flowability of mixed powders based on the lower HR, CI, and SAoR. e remaining experiments, E1, E2, E3, E5, E6, E7, E11, E16, E17, E18, E19, and E20, exhibit fair flow characteristics. From the observations, irrespective of varying NbC composition, it was clear that the factor-based experiments yielded a good flow for the mixed powders owing to the proper set of input parameters, except for E1, E2, and E7. ese experiments also exhibit good HR and CI, but the angle of repose is high due to the nonuniform dispersion of NbC particles, affecting the flow and inducing a frictional effect between the reinforcement and matrix. Moreover, the center-based and extreme-based experiments do not yield satisfactory results, except for experiment E13, because the mixing occurs at a higher speed of 234.05 RPM.    Hausner ′ s Ratio(HR) �

Tapped Density Apparant Density
Static Angle of Repose(SAoR), tan θ � 2 × Height of the Piling (H in mm) Base Diameter of the Piling (D in mm) . (3) e center-based, extreme-based, and factor-based scanning electron microscope (SEM) images are shown in respectively. e SEM images of the mixed powder under various input parameters were used to ensure the morphology of the AlSi10Mg with NbC and the distribution of the reinforcement (NbC) in the matrix (AlSi10Mg). Figures 3-5 depict that the AlSi10Mg morphology is not modified, and NbC particles' presence was observed. Here, the yellow circle is used to indicate the presence of NbC particles in the matrix.

Percentage Contribution of Input Parameters for
Responses. Table 4shows the statistical values based on the full quadratic model. e values depict that the model is adequate for analysis and further experimentation. If the p value and F-value are less than 0.05 and greater than 4, respectively, at a 95 percent confidence level, the proposed model is significant, and the corresponding input parameter is taken into account for the output response. e model's R square value for all responses was greater than 90 percent, which reveals that the model could explore 90 percent of the possible changes in the output responses. e model can significantly predict the process if the R square and adjusted R square values are greater than 80 percent. e input parameters, such as speed and NbC composition, contribute more substantially to the responses, such as apparent density and tapped density. e most vital input parameter affecting the static angle of repose is speed. Also, the interaction of time and NbC composition contributes to the static angle of repose.

Validation of Regression Equation.
e regression equations (4)-(6) were used to predict output responses such as apparent density, tapped density, and static angle of repose by including quadratic terms of linear, square, and two-way interaction of input parameters. e residual value was obtained from the difference between experimented and predicted data. If the residual values are small, the proposed regression equations are accurate. Table 5 shows the residual values for the responses, depicting that the fitted data are close to the experimented data. So, the proposed regression equations have verified the adequacy of the full quadratic model.              Advances in Materials Science and Engineering 9 tapped densities with the minimum static angle of repose. e maximum apparent density ensures that the mixed powders are not entirely irregular in morphology, introduce smaller particles (NbC) between the AlSi10Mg particles, and have low pores in the initial packed density. e particles' cohesiveness was controlled, establishing good flow to the mixed powder at maximum tapped density criteria. Based on the maximum condition of both densities, low HR and CI were attained. ese values ensure good flowability characteristics. Finally, the minimum static angle of repose confirms the low cohesiveness and minimum frictional effect during the powder flow. e static angle of repose is inversely proportional to the flowability of the mixed powder. Table 6 shows the goal of the output responses with importance and weight, along with constraint values. Figure 9 displays the optimal results with a composite desirability limit to address the multiple objective output response by pulling out the higher and lower point from the 3D surface plot concerning the defined objective. e optimum condition is as follows: time � 1.95 hours, speed � 71.50 RPM, NbC composition � 8% weight. e predicted values of apparent density, tapped density, and static angle of repose are 1.3317 g/cc, 1.5333 g/cc, and 0.3887 radians (22.17 degrees) with composite desirability of 0.897.
As shown in Figure 10,the validation experiment was carried out under optimized conditions for the confirmatory purpose, and the experimental data were compared with predicted data, as shown in Figure 10. From Figure 11, it was observed that there was no change in the matrix (AlSi10Mg) morphology and tiny satellites on the surface of the matrix.

Conclusion
In this experimental investigation, the CCD was employed to predict the processing conditions for regular mixing of AlSi10Mg and NbC. From the experimental analysis, the following points can be observed: (1) e factor-based experiments show promising results based on flowability characteristics when compared to center-based and extreme-based experiments (2) Based on the SEM images, the morphology of the matrix element (AlSi10Mg) had not been changed after being mixed with varying percentages of NbC at a different set of parameters, and proper distribution of NbC was observed. (3) e apparent and tapped density ratio was insufficient for predicting the flow of mixed powder. Another response is also required to assess the flow characteristics. So, the static angle of repose was employed to predict the mixed powder's cohesiveness despite its low HR and CI values. e undesired flow characteristics were observed at a high percentage of NbC and the extended mixing time. (4) e optimum condition of input parameters reveals that the low-speed mixing was preferable to achieve maximum apparent and tapped densities with the minimum static angle of repose. (5) Finally, the optimized combination of mixed powder (AlSi10Mg + 8% weight of NbC) was attained, showing good flowability characteristics. Furthermore, it satisfies the processability criteria of additive manufacturing.

Data Availability
e data used to support the findings of this study are included in the article.

Conflicts of Interest
e authors declare that there are no conflicts of interest regarding the publication of this paper.